bluuebunny/crossref_metadata_2025 huggingface dataset:
Brittle Fracture of a Marine Riser Clamp
Authors: Mahmoud Salah E.
Published: May 2019

An API type 2 steel clamp located on the riser of a semisubmersible drilling rig between the lower ball joint and riser blowout preventer (BOP) conductor failed after 7 years of service. Failure analysis revealed the cause of failure to be the low toughness of the clamp material. Contributing factors included the presence of a hard, brittle, heat-affected zone and weld defects at the handling pad eye. It was recommended that the replacement clamp be made from a material with good toughness and that any installation of attachments by welding be done according to qualified procedures.
Failure of 9% Ni Steel Production Tubing
Authors: Billings Robert M.
Published: May 2019

During a work over of an oil well, the 9% Ni steel production tubing parted three times as it was being pulled from the well. The tubing had performed satisfactorily for more than 30 years in the well A representative failure, a circumferential fracture in a connection, was analyzed. Reported to be a hydril CS connection, the pin end parted near the last threads. The external surface exhibited mechanical damage marks from the fishing operation. No signs of external corrosion or damage were detected. Visual surface examination revealed shear lips at the outside pipe, indicating that the fracture initiated at the inside surface and grew across the wall. Longitudinal cross sections revealed heavy corrosion damage to the inside pipe surface. Metallographic examination indicated that the tubing failed as a result of severe weakening from internal corrosion. Gray-colored corrosion deposits, which penetrated the pipe throughout the grain boundaries of the material and concentrated in the matrix in a layer near the inside surface of the pipe, were observed. The presence of H2S in the produced fluids and the appearance of the gray deposit indicated that the tube suffered H2S corrosion. Chemical analysis of the base metal and corrosion deposits did not detect iron or nickel sulfides, however Replacement of the remaining pipe strings according to a scheduled program was recommended. Because 9% Ni steel was not available, 13% Cr martensitic stainless steel was recommended as a replacement.
Failure of Stainless Steel Springs Used in an Oil Ring Lip Seal
Authors: Neff Michael
Published: May 2019

Failure of AISI type 321 stainless steel internal springs from newly manufactured lip seals on a shaft between a turbine power unit and a pump in a commercial aircraft secondary unit was investigated. Examination of the coils from two failed springs showed that both had failed by fatigue. The springs contained drawing defects that served as the fatigue crack initiation sites. It was recommended that the wire drawing process be investigated for various levels of steel cleanliness to predict the incidence of drawing defects at the wire surface. Stress analysis to determine the minimum tolerable defect size was also recommended.
Sledgehammer Chipping Failure
Authors: Garber Richard
Published: May 2019

A sledge hammer chipped during use. The chip struck a by stander in the eye, leading to its loss. The hammerhead surface was examined visually, nondestructively (magnetic particle method), and stereo microscopically, and a microstructural analysis of a cross section of the head was conducted using optical microscope. Chemical composition of the hammerhead was determined by emission spectrometry. The chemical compositions of the chip and hammer head were compared using energy-dispersive analysis. Microhardness versus distance from the striking face was also determined. The hammerhead material was UNS G10800 (AISI/SAE grade 1080). Excessive hardnesses were measured in the first 3 mm (0. 12 in.) below the striking surface, indicating that there was lack of control during the final tempering operation.
Fatigue Fracture of Aluminum Wires in High-Voltage Electrical Cables in Alaska
Authors: Chakrapani Durgam G.
Published: May 2019

Several wires in aluminum conductor cables fractured within 5 to 8 years of, service in Alaskan tundra. The cables were comprised of 19-wire strands; the wires were aluminum alloy 6201-T81. Visual and metallographic examinations of the cold-upset pressure weld joints in the wires established that the fractures were caused by fatigue loading attributable to wind/thermal factors at the joints. The grain flow at the joints was transverse to the wire axis, rendering the notches of the joints sensitive to fatigue loading. An additional contributory factor was intergranular corrosion, which assisted fatigue crack initiation/propagation. The failure was attributed to the departure of conductor quality from the requirements of ASTM B 398 and B 399, which specify that “no joints shall be made during final drawing or in the finished wire” and that the joints should not be closer than 15 m (50 ft). The failed cable did not meet either criterion. It was recommended that the replacement cable be inspected for strict compliance to ASTM requirements.
Delayed Fracture of Tempered Glass Panels Due to Nickel Sulfide Inclusions
Authors: Huet Roland , Wolf Joel M. , Moncarz Piotr D.
Published: May 2019

The spontaneous breakage of tempered glass spandrel panels used to cover concrete wall panels on building facades was investigated. Between January 1988 and August 1990, 19 panel failures were recorded. The tinted panels were coated on their exterior surfaces with a reflective metal oxide and covered on the back surfaces with an adherent black polyethylene plastic. Macro fractography, SEM fractography, EDX analysis, and photo elasticimetry were conducted on four of the shattered panels. Small nickel sulfide inclusions were found at the failure origins. Failure of the panels was attributed to growth of the inclusions, coupled with high residual stresses. Fracture mechanics analysis showed that the residual stresses alone were high enough to cause fracture of the glass, with a flaw of the size observed.
Failure of a Cast Steel Crane Bolster
Authors: Stone Alan
Published: May 2019

The failure of a 45 Mg (50 ton) rail crane bolster was investigated. Spectrochemical analysis indicated that the material was a 0.25C-1.24Mn-0.62Cr-0.24Mo cast steel. SEM examination revealed the presence of fatigue, as well as intergranular and ductile fractures. Microstructural analysis focused on an area where an antisway device had been welded to the structure and revealed the presence of coarse, untempered martensite that had resulted from faulty weld repair techniques. It was suggested that the use of proper welding procedures, including preheating and postheating, would have prevented the failure.
Spalling of a Ball-Peen Hammer
Authors: D'Antonio Carmine
Published: May 2019

A carbon steel ball-peen hammer ejected a chip that struck the user's eye. Failure occurred when two hammers were struck together during an attempt to free a universal joint from an automotive drive shaft. Two samples were cut from the face of the hammer one through the chipped area on the chamfer and the other from the undamaged area on the chamfer. The shape and texture of the fracture surfaces were typical of spalling. The fracture was conchoidal and exhibited a complete lack of plastic deformation. White etching bands that intersected the face and chamfer were revealed during metallographic examination. Fracture occurred through a white band. Failure was attributed to formation of envelopes of untempered martensite under the chamfer that ruptured explosively during service.
Corrosion Failure of Stainless Steel Components During Surface Pretreatment
Authors: Dayal R.K. , Gnanamoorthy J.B. , Division Metallurgy , Srinivasan G.
Published: May 2019

Two AISI type 316 stainless steel components intended for use in a reducer section for sodium piping in a fast breeder test reactor were found to be severely corroded—the first soon after pickling, and the second after passivation treatments. Metallographic examination revealed that one of the components was in a highly sensitized condition and that the pickling and passivation had resulted in severe intergranular corrosion. The other component was fabricated from thick plate and, after machining, the outer surface represented the transverse section of the original plate. Pickling and passivation resulted in severe pitting because of end-grain effect. Strict control of heat treatment parameters to prevent sensitization and modification of pickling and passivating conditions for machined components were recommended.
Cracking During Forging of Extruded Aluminum Alloy Bar Stock Material
Authors: Das A.K.
Published: May 2019

During the preproduction stages of forging, an initial batch of 50 mm (2 in.) diam Al-4Cu alloy (L77) extruded bar stock material was found to be cracking randomly. Failure analysis was conducted to determine the metallurgical factors underlying the phenomenon. Microexamination of sections across the defects revealed intergranular cracks tracing a path of round, segregated particles and oxide film discontinuities. The segregated particles were rich in copper It was concluded that the cracking was the result of segregations occurring in poor-quality raw material. The source of segregation was suspected to be the use of improperly made master alloys. Use of improved melting techniques and proper master alloys was recommended.
Failure of Compound Bow Handle Risers
Authors: Goodrich George M.
Published: May 2019

Compound bow handle risers that had failed in service and during assembly along with an unassembled riser were submitted for analysis. The risers were die cast from magnesium-base alloy AM60A. Inspection of the failed risers and metallurgical investigations conducted on the stock riser revealed the presence of cold shuts at the same site in all specimens. It was recommended that all risers be thoroughly inspected and that the bow company work with their die casting shop to design a mold with acceptable filling characteristics.
Fatigue Fracture of a Helicopter Tail Rotor Blade Due to Field-Induced Corrosion
Authors: McSwain Richard H.
Published: May 2019

A helicopter tail rotor blade spar failed in fatigue, allowing the blade to separate during flight. The 2014-T652 aluminum alloy blade had a hollow spar shank filled with lead wool ballast and a thermoset polymeric seal. A corrosion pit was present at the origin of the fatigue zone and numerous trails of corrosion pits were located on the spar cavity's inner surfaces. The corrosion pitting resulted from the failure of the thermoset seal in the spar shank cavity. The seal failure allowed moisture to enter into the cavity. The moisture then served as an electrolyte for galvanic corrosion between the lead wool ballast and the aluminum spar inner surface. The pitting initiated fatigue cracking which led to the spar failure.
Processing-Induced Fatigue Fracture of a Helicopter Tail Rotor Blade
Authors: McSwain Richard H.
Published: May 2019

A helicopter tail rotor blade spar failed in fatigue, allowing the outer section of the blade to separate in flight. The 7075-T7351 aluminum alloy blade had fiberglass pockets. The blade spar was a hollow “D” shape, and corrosion pits were present on the inner surface of the hollow spar A single corrosion pit, 0.38 mm (0.015 in.) deep, led to a fatigue failure of the spar The failure initiated on the pylon side of the blade. Dimensional analysis of the spar near the failure revealed measurements within engineering drawing tolerances. Though corrosion pitting was present, there was an absence of significant amounts of corrosion product and all of the pits were filled with corrosion-preventative primer. This indicated that the pitting occurred during spar manufacture, prior to the application of the primer The pitting resulted from multiple nickel plating and defective plating removal by acid etching. Post-plating baking operations subsequently reduced the fatigue strength of the spar.
Fatigue Fracture of a Transport Aircraft Crankshaft During Flight
Authors: Das A.K.
Published: May 2019

A 4340 steel piston engine crankshaft in a transport aircraft failed catastrophically during flight. The fracture occurred in the pin radius zone. Fractographic studies established the mode of failure as fatigue under a complex combination of bending and torsional stresses. SEM examination revealed that the fracture origin was a subsurface defect-a hard refractory (Al2O3) inclusion—in the zone close to the pin radius. Chemical analysis showed the crankshaft material to be of inferior quality. It was recommended that magnetic particle inspection using the dc method be used to cheek for cracks during periodic maintenance overhauls.
Contact Fatigue Failure of A Bull Gear
Authors: Tanner G. Mark , Harty James R.
Published: May 2019

A bull gear from a coal pulverizer at a utility failed by rolling-contact fatigue as the result of continual overloading of the gear and a nonuniform, case-hardened surface of the gear teeth. The gear consisted of an AISI 4140 Cr-Mo steel gear ring that was shrunk fit and pinned onto a cast iron hub. The wear and pitting pattern in the addendum area of the gear teeth indicated that either the gear or pinion was out of alignment. Beach marks observed on the fractured surface of the gear indicated that fatigue was the cause of the gear failure. Similar gears should be inspected carefully for signs of cracking or misalignment. Ultrasonic testing is recommended for detection of subsurface cracks, while magnetic particle testing will detect surface cracking. Visual inspection can be used to determine the teeth contact pattern.
Failure of Four Cast Steel Gear Segments
Authors: Goodrich George M.
Published: May 2019

Gears in a strip mining dragline failed in service. The material was identified as a low-alloy (NiCrMoV) steel. SEM analysis indicated that the initial fracture and subsequent fractures resulted from impact or a suddenly applied load. Mechanical testing indicated that the gears had low impact strength. Failure was attributed to low toughness caused by the absence of, or improper, heat treatment. Casting defects identified during metallographic examination were determined to be the fracture initiation site, but were considered less significant than the low as-received impact strength of the material. It was recommended that the equipment manufacturer implement an appropriate heat treatment to meet the impact requirements of the application.
Three-Wheel Motorcycle Frame Failures and Redesign
Authors: Knott Thomas A.
Published: May 2019

Bending fatigue caused crack propagation and catastrophic failures at several locations near the welds on the low-carbon steel tubular cargo box frame of police three-wheel motorcycles. ANSYS finite element analysis revealed that bending stresses in some of the frame members were aggravated by poor detail design between vertical and horizontal tubes. Stresses observed in the ANSYS analysis were not sufficient to cause the onset of fatigue. However when compounded by stress concentration factors and in-service dynamic loading, the frame could have been regularly subjected to stresses over the fatigue limit of the material. A strain gage static loading test verified FEM results, and finite element techniques were applied in the design of reinforcing members to renovate the frames. Material properties were determined and welding procedures specified for the reinforcing members. Inspection intervals were devised to avoid future problems.
Failure of Admiralty Brass Condenser Tubes
Authors: Khatak H.S. , Gnanamoorthy J.B. , Rodriguez P.
Published: May 2019

Leaks developed in 22 admiralty brass condenser tubes. The tubes were part of a condenser that was being used to condense steam from a nuclear power plant and had been in operation for less than 2 years. Analysis identified three types of failure modes: stress-corrosion cracking, corrosion under deposit (pitting and crevice), and dezincification. Fractures were transgranular and typical of stress-corrosion cracking. The primary cause of the corrosion deposit was low-flow conditions in those parts of the condenser where failure occurred. Maintenance of proper flow conditions was recommended.
Failure of Three Cyclone Separators
Authors: Goodrich George M.
Published: May 2019

Three 1006 carbon steels team/water separators failed in a boiler in installation after several years of service. Annual inspection had revealed no evidence of deterioration until the last inspection, when they were removed from service. Metallurgical investigation determined that the separators had deteriorated because of erosion corrosion. Further analysis of the boiler operation revealed that operational changes made in the last year of service caused an increase in velocity of the water/steam mixture. It was recommended that the operating parameters for the boiler be reevaluated and prior levels of operation be reinstituted.
Intergranular Stress-Corrosion Cracking Failure in AISI Type 316 Stainless Steel Dished Ends Near Weld Joints
Authors: Bhattacharya D.K. , Jayakumar T. , Raj Baldev
Published: May 2019

Two AISI type 316 stainless steel dished ends failed through the formation of intergranular stress-corrosion cracks (IGSCC) within a few months of service. The dished ends failed in the straight portions near the circumferential welds that joined the ends to the cylindrical portions of the vessel. Both dished ends were manufactured from the same batch and were supplied by the same manufacturer One of the dished ends had been exposed to sodium at 550 deg C (1020 deg F) for 500 h before failure due to sodium leakage was detected. The other dished end was used to fabricate a second vessel that was kept in storage for 1 year Clear evidence of sensitization was found in areas where IGSCC occurred. Sensitization was extensive in the dished end that had been exposed to sodium at high temperature, and it occurred in a narrow band similar to that typical of weld decay in the dished end that had been kept in storage. Solution annealing was recommended to relieve residual stress, thereby reducing the probability of failure. It was also recommended that the carbon content of the steel be lowered, i.e., that a 316L grade be used.
Alkaline-Type Boiler Tube Failures Induced by Phosphate Water Treatment
Authors: Islam Moavinul
Published: May 2019

Tube failures occurred in quick succession in two boiler units from a bank of six boilers in a refinery. The failures were confined to the SAE 192 carbon steel horizontal support tubes of the superheater pack. In both cases, the failure was by perforation adjacent to the welded fin on the crown of the top tubes and located in an area near the upward bend of the tube. The inside of all the tubes were covered with a loosely adherent, black, alkaline, powdery deposit comprised mainly of magnetite. The corroded areas, however, had relatively less deposit. The morphology of the corrosion damage was typical of alkaline corrosion and confirmed that the boiler tubes failed as a result of steam blanketing that concentrated phosphate salts. The severe alkaline conditions developed most probably because of the decomposition of trisodium phosphate, which was used as a water treatment chemical for the boiler feed water.
Caustic-Induced Stress-Corrosion Cracking of a Flue Gas Expansion Joint
Authors: Hahn Sarah Jane
Published: May 2019

A type 430Ti stainless steel flue gas expansion joint cracked because of caustic-induced stress-corrosion cracking. Energy-dispersive X-ray spectroscope analysis of the fracture surface deposits revealed the presence of sodium and potassium—caustics in hydroxide form. Primary fracture surfaces were all similar in appearance, and a primary crack origin could not be identified. A secondary crack brought to fracture in the laboratory showed brittle, cleavage features rather than classic, tensile overload features. This suggested that the material was embrittled.
Failure of Carbon Steel Superheater Tubes
Authors: Ribble Joseph P.
Published: May 2019

Two superheater tubes from a 6.2 MPa (900 psig) boiler failed in service because of creep rupture. One tube was carbon steel and the other was carbon steel welded to ASTM A213 Grade T22 (2.25Cr-1.0Mo) tubing. The failure in the welded tube occurred in the carbon steel section. Portions of the superheater were retubed five years previously with Grade 722 material. The failures indicated that tubes were exposed to long-term overheating conditions. While the carbon steel tube did not experience temperatures above the lower transformation temperature 727 deg C (1340 deg F), the welded tube did experience a temperature peak in excess of 727 deg C (1340 deg F). The long-term overheating conditions could have been the result of excessive heat flux and /or inadequate steam flow. In addition, the entire superheater bank should have been upgraded to Grade 722 material at the time of retubing.
Failure of a Pipe Slip-on Flange
Authors: Chaudhari Mohan D.
Published: May 2019

A cracked 356 mm (14 in.) diam slip-on flange (Ni-Cr-Mo-V steel) was submitted for failure analysis. Reported results and observations indicated that the flange was not an integral forging or a casting, as specified. It had been fabricated by welding and machining a ring insert within a flange with a larger internal diameter. The flange cracked because the welds between the flange and the insert were inadequate to withstand the bolting pressures. A warning was issued to end users of the flanges, which are being inspected nondestructively for conformance to specifications.
Graphitization-Related Failure of a Low-Alloy Steel Superheater Tube
Authors: Kotwica David J.
Published: May 2019

A carbon-molybdenum (ASTM A209 Grade T1) steel superheater tube section in an 8.6 MPa (1250 psig) boiler cracked because of long-term overheating damage that resulted from prolonged exposure to metal temperatures between 482 deg C (900 deg F) and 551 deg C (1025 deg F). The outer diameter of the tube exhibited a crack (fissure) oriented approximately 45 deg to the longitudinal axis and 3.8 cm (1.5 in.) long. The inner diameter surface showed a fissure in the same location and orientation. Microstructure at the failure near the outer diameter surface exhibited evidence of creep cracking and creep void formation at the fissure. A nearly continuous band of graphite nodules was observed on the surface of the fissure. In addition to the graphite band formation, the microstructure near the failure exhibited carbide spheroidization from long-term overheating in all the tube regions examined. It was concluded that preferential nucleations of graphite nodules in a series of bands weakened the steel locally, producing preferred fracture paths. Formation of these graphite bands probably expedited the creep failure of the tube. Future failures may be avoided by using low-alloy steels with chromium additions such as ASTM A213 Grade T11 or T22, which are resistant to graphitization damage.
Stress-Corrosion Cracking of Stainless Steel Superheater Tubing
Authors: Esmacher Mel J.
Published: May 2019

Several 304H stainless steel superheater tubes fractured in stressed areas within hours of a severe caustic upset in the boiler feedwater system. Tests performed on a longitudinal weld joint, which connected two adjacent tubes in the tertiary superheater bank, confirmed caustic-induced stress-corrosion cracking, promoted by the presence of residual welding stresses. Improved maintenance of check valves and routine inspection of critical monitoring systems (conductivity alarms, sodium analyzers, etc.) were recommended to help avoid future occurrences of severe boiler feedwater contamination. Additional recommendations were to eliminate these short longitudinal weld joints by using a bracket assembly joint between the tubes, use a post-weld heat treatment to relieve residual welding stress or select a more stress-corrosion cracking resistant alloy for this particular application.
Stress-Corrosion Cracking of a Swaged Stainless Steel Reheater Pendent Tube
Authors: Studer Anthony C. , Dickens Robert S.
Published: May 2019

A cold-formed Grade TP 304 stainless steel swaged region of a reheater tube in service for about 8000 hours cracked because of sulfur-induced stress-corrosion cracking (SCC). Cracking initiated from the external surface and a high sulfur content was detected in the outer diameter and crack deposits. Comparison of the microstructure and hardness of the swaged region and unswaged Grade TP 304 stainless steel tube metal indicated that the swaged section was not annealed to reduce the effects of cold working. The high hardness created during swaging increased the stainless steel's susceptibility to sulfur-induced SCC. Because SCC requires water to be present, cracking most likely occurred during downtime or startups. To prevent future failures, the boiler should be kept dry during downtime to avoid formation of sulfur acids, and the swaged sections of the tubes should be heat treated after swaging to reduce or eliminate strain hardening of the metal.
Brittle Fracture Explosive Failure of a Pressurized Railroad Tank Car
Authors: Brown Samuel J.
Published: May 2019

A 127 cu m (4,480 cu ft) pressurized railroad tank car burst catastrophically. The railroad tank was approximately 18 m (59 ft) long (from 2:1 elliptical heads), 3 m (10 ft) in OD, and 16 mm (0.63 in.) thick. The chemical and material properties of the tank were to comply with AAR M-128 Grade B. As a result of the explosive failure of the tank car, fragments were ejected from the central region of the car between the support trucks from ground zero to a maximum of approximately 195 m (640 ft). The mode of failure was a brittle fracture originating at a preexisting lamination and crack in the tank wall adjacent to the tank nozzle. The mechanism of failure was overpressurization of the railroad tank car caused by a chemical reaction of the butadiene contents. The interrelationship of the mode, mechanism, and consequences of failure is reviewed to reconstruct the sequence of events that led up to the breach of the railroad tank car. Means to prevent similar reoccurrences are discussed.
Fatigue Failure at Fillet-Welded Nozzle Joints in a Type 316L Stainless Steel Tank
Authors: Bhattacharya D.K. , Ray S.K. , Rodriguez Placid
Published: May 2019

Upon arrival at the erection site, an AISI type 316L stainless steel tank intended for storage of fast breeder test reactor coolant (liquid sodium) exhibited cracks on its shell at two of four shell/nozzle fillet-welded joint regions. The tank had been transported from the manufacturer to the erection site by road, a distance of about 800 km (500 mi). During transport, the nozzles were kept at an angle of 45 deg to the vertical because of low clearance heights in road tunnels. The two damaged joints were unsupported at their ends inside the vessel, unlike the two uncracked nozzles. Surface examination showed ratchet marks at the edges of the fracture surface, indicating that loading was of the rotating bending type. Electron fractography using the two-stage replica method revealed striation marks characteristic of fatigue fracture. The striations indicated that the cracks had advanced on many “mini-fronts,” also indicative of nonuniform loading such as rotating bending. It was recommended that a support be added at the inside end of the nozzles to rigidly connect with the shell. In addition to avoiding transport problems, this design modification would reduce fatigue loading that occurs in service due to vibration of the nozzles during filling and draining of the tank.
Failure of a Martensitic Stainless Steel Ball Valve
Authors: Kaul Rakesh , Muralidharan N.G. , Kasiviswanathan K.V. , Raj Baldev
Published: May 2019

Repeated failures of high-pressure ball valves were reported in a chemical plant. The ball valves were made of AFNOR Z30C13 martensitic stainless steel. Initial examination of the valves showed that failure occurred in a weld at the ball/stem junction end of austenitic stainless steel sleeves that had been welded to the valve stem at both ends. Metallographic examination showed that a crack had been introduced into the weld by improper weld heat treatment. Stress concentration at the weld location resulting from an abrupt change in cross section facilitated easy propagation of the crack during operation. Proper weld heat treatment was recommended, along with avoidance of abrupt change in cross section near the weld. Due penetrant testing at the ball stem junction before and after heat treatment was also suggested.
Cracking in a Steam Turbine Rotor Disk
Authors: Colwell Richard L.
Published: May 2019

An A-470 steel rotor disk was removed from the high-pressure portion of a steam turbine-powered compressor after nondestructive testing revealed cracks in the shoulder of the disk during a scheduled outage. Samples containing cracks were examined using various methods. Multiple cracks, primarily intergranular were found on the inlet and outlet faces along prior-austenite grain boundaries. The cracks initiated at the surface and propagated inward. Multiple crack branching was observed. Many of the cracks were filled with iron oxide. X-ray photoelectron spectroscopy indicated the presence of sodium on crack surfaces, which is indicative of NaOH-induced stress-corrosion cracking. Failure was attributed to superheater problems that resulted in caustic carryover from the boiler. Two options for disk repair, installing a shrink-fit disk or applying weld buildup, were recommended. Weld repair was chosen, and the rotor was returned to service; it has performed for more than 1 year without further incident.
Failure Analysis of a Cracked Low-Pressure Turbine Blade
Authors: Ciulik J.
Published: May 2019

A cracked, martensitic stainless steel, low-pressure turbine blade from a 623 MW turbine generator was found to exhibit fatigue cracks during a routine turbine inspection. The blade was cracked at the first notch of the fir tree and the cracks initiated at pits induced by chloride attack. Examination of the blade microstructure at the fracture origins revealed oxide-filled pits and transgranular cracks. The oxide filled cracks appeared to have originated at small surface pits and probably propagated in a fatigue or corrosion-fatigue fracture mode. It was recommended that the sources of the chlorides be eliminated and that the remaining blades be inspected at regular maintenance intervals for evidence of cracking.
Failure of Non-Magnetic Retaining Ring in a High-Speed Generator Rotor
Authors: Sherlock Thomas P. , Jirinec Michael J.
Published: May 2019

A shrunk-fit 18 Mn-5Cr steel retaining ring failed without warning during normal unit operation of a 380 MW electrical generator. The cause of the ring failure was determined to be intergranular stress-corrosion cracking (IGSCC) because of the high strength of the ring material and the presence of moist hydrogen used to cool the ring. Factors which promoted the failure were higher than normal strength levels in the ring material, lower than normal ring operating temperatures, possible moisture in the lubrication oil system, periodic poor performance of the hydrogen dryers, and a ring design which allowed water to become trapped in a relief groove. These factors caused pitting in the ring in an estimated 100 hours of operation. The ring had been inspected previously 18 months prior to the failure and no defects or pitting were found. Calculations showed that a 0.127-cm (0.050-in.) deep pit could grow to a critical size in 3000 to 4000 hours of operation. To prevent further failures, it was recommended that the ring be replaced with an 18 Mn-18Cr alloy with superior resistance to IGSCC. A program of periodic inspection and replacement of other retaining rings in the system was also recommended.
Fatigue Cracking of Gas Turbine Diaphragms
Authors: Fleck N.A.
Published: May 2019

Several compressor diaphragms from five gas turbines cracked after a short time in service. The vanes were constructed of type 403 stainless steel, and welding was performed using type 309L austenitic stainless steel filler metal. The fractures originated in the weld heat-affected zones of inner and outer shrouds. A complete metallurgical analysis was conducted to determine the cause of failure. It was concluded that the diaphragms had failed by fatigue. Analysis suggests that the welds contained high residual stresses and had not been properly stress relieved. Improper welding techniques may have also contributed to the failures. Use of proper welding techniques, including appropriate prewelding and postwelding heat treatments, was recommended.
Fatigue Fracture of a Precipitation-Hardened Stainless Steel Actuator Rod End
Authors: Levy Eli
Published: May 2019

A 17-4 PH steering actuator rod end body broke during normal take-off. Results of failure analysis revealed that the wall thickness of the race was much below the design limits, thus causing the race to rest on the body's swaged edges rather than on the load carrying centerline of the body. This assembly condition generated abnormal high loads on the swaged edges, ultimately resulting in fatigue failure. To prevent a recurrence of similar failure in the future, the dimensions of the race in the spherical bearing were changed, no further failure occurred.
Metallurgical Analysis of Steam Turbine Rotor Disc
Authors: Hodas Leonard J.
Published: May 2019

Numerous cracks observed on the surface of a forged A470 Class 4 alloy steel steam turbine rotor disc from an air compressor in a nitric acid plant were found to be the result of caustic induced stress-corrosion cracking (SCC). No material defects or anomalies were observed in the disc sample that could have contributed to crack initiation or propagation or secondary crack propagation. Chlorides detected in the fracture surface deposits were likely the primary cause for the pitting observed on the disc surfaces and within the turbine blade attachment area. It was recommended that the potential for water carryover or feedwater induction into the turbine be addressed via an engineering evaluation of the plant's water treatment procedures, steam separation equipment, and start-up procedures.
Failure of a Crane Long-Travel Worm Drive Shaft
Authors: Wellington K.G.
Published: May 2019

A crane long-travel worm drive shaft was found to be chipped during unpacking after delivery. Chemical analysis showed that the steel (EN36A with a case depth of 1 mm, or 0.04 inch did not meet specifications. Magnetic particle inspection revealed a crack on the side of the shaft opposite the chip. Metallographic examination indicated that the case depth was approximately 2 mm (0.08 in.) and that a repair weld of an earlier chip had been made in the cracked area. The chipping was attributed to excessive case depth and rough handling. It was recommended that the shaft be returned to the manufacturer and a replacement requested.
Fatigue Failure of a Circulating Water Pump Shaft
Authors: Hare Joyce M.
Published: May 2019

A type 410 stainless steel circulating water pump shaft used in a fossil power steam generation plant failed after more than 7 years of service. Visual examination showed the fracture surface to be coated with a thick, spalling, rust-colored scale, along with evidence of pitting. Samples for SEM fractography, EDS analysis, and metallography were taken at the crack initiation site. Hardness testing produced a value of approximately 27 HRC. The examinations clearly established that the shaft failed by fatigue. The fatigue crack originated at a localized region on the outside surface where pitting and intergranular cracking had occurred. The localized nature of the initial damage indicated that a corrosive medium had concentrated on the surface, probably due to a leaky seal. Reduction of hardness to 22 HRC or lower and inspection of seals were recommended to prevent future failures.
Fracture of a Coupling in a Line-Shaft Vertical Turbine Pump
Authors: Eryürek I.B. , Aran A. , Capa M.
Published: May 2019

A coupling in a line-shaft vertical turbine pump installed in a dam foundation fractured after a very short time. The coupling material was ASTM A582 416 martensitic stainless steel. Visual, macrofractographic, and scanning electron microscopic examination of the coupling showed that the fracture was brittle and was initiated by an intergranular cracking mechanism. The mode of fracture outside the crack initiation zone was transgranular cleavage. No indication of fatigue was found. The failure was attributed to improper heat treatment during manufacture, which resulted in a brittle microstructure susceptible to corrosion. The crack initiated either by stress-corrosion or hydrogen cracking. It was recommended that the couplings in the system be examined for surface cracking and, if present, corrective measures be taken.
Anomalous Fractures of Diesel Engine Bearing Cap Bolts
Authors: Walter G.H. , Hendrickson R.M. , Zipp R.D.
Published: May 2019

Sudden and unexplained bearing cap bolt fractures were experienced with reduced-shank design bolts fabricated from 42 CrMo 4 steel, quenched and tempered to a nominal hardness of 38 to 40 HRC. Fractographic analysis provided evidence favoring stress-corrosion cracking as the operating transgranular fracture failure mechanism. Water containing H7S was subsequently identified as the aggressive environment that precipitated the fractures in the presence of high tensile stress. This environment was generated by the chemical breakdown of the engine oil additive and moisture ingress into the normally sealed bearing cap chamber surrounding the bolt shank. A complete absence of fractures in bolts from one of the two vendors was attributed primarily to surface residual compressive stresses produced on the bolt shank by a finish machining operation after heat treatment. Shot cleaning, with fine cast shot, produced a surface residual compressive stress, which eliminated stress-corrosion fractures under severe laboratory conditions.
Failed Bolts From an Army Tank Recoil Mechanism
Authors: Champagne Victor K.
Published: May 2019

The heads of two AISI 8740 steel bolts severed while being installed into an Army tank recoil mechanism. Both broke into two pieces at the head-to-shank radius and the required torque value had not been attained nor exceeded prior to the failure. A total of 69 bolts from inventory and the field were tested by magnetic particle inspection. One inventory bolt failed because of a transverse crack near the head-to-shank radius. It was deduced that either a 100% magnetic particle inspection had not been conducted during bolt manufacturing, or the crack went undetected during the original inspection. Optical and electron microscopy of the broken bolts revealed topographies and the presence of black oxide consistent with quench cracking. The two bolts failed during installation due to the presence of pre-existing quench cracks. Recommendations to prevent future failures include: ensuring that 100% magnetic particle inspections are conducted after bolts are tempered; using dull cadmium plate or an alternative to the electrode position process, such as vacuum cadmium plate or ion-plate or ion-plated aluminum, to mitigate the potential for delayed failures due to hydrogen embrittlement or stress-corrosion cracking; ensuring that the radius at the shoulder/shank interface conforms to specifications; and replacing all existing bolts with new or reinspected inventory bolts.
Failed Main Rotor Pitch Horn Bolt from an Army Attack Helicopter
Authors: Champagne Victor K. , Pepi Marc , Wechsler Gary
Published: May 2019

One of the two AISI 4340 steel pitch horn bolts from the main rotor hub assembly failed while in service. Optical microscope revealed evidence of corrosion pitting in regions adjacent to the fracture. Fractographic examination utilizing a scanning electron microscope revealed multiple crack origins which assumed a “thumbnail” shape and displayed surface morphologies which resulted from intergranular decohesion. Many of the crack sites initiated from corrosion pits. Energy dispersive spectroscope performed on areas within the crack initiation site showed the presence of chlorides. The failure was attributed to stress-corrosion cracking. Short- and long-term recommendations to prevent future failures are given.
Arcing Fault Burndown in Low Voltage Residential Service Entrance with Aluminum Conductors
Authors: Prosser Howard F. , Shipley Roch J. , Bouldin Peter C.
Published: May 2019

Three instances involving the failure of aluminum wiring at the service entrance to single-family homes are discussed. Arcing led to a fire which severely damaged a home in one case. In a second, the failure sequence was initiated by water intrusion into the service entrance electrical box during construction of the home. In the third, failure was caused by a marginal installation. Strict adherence to all applicable electrical codes and standards is critical in the case of aluminum wiring. Electrical components not specifically designed for aluminum must never be used with this type of wiring. All doors, panels and similar portions of electrical boxes should be secured to prevent damage to surroundings in the event of an electrical fault. If symptoms of arcing are observed, professional service should be sought. The latest designs of connectors for use with aluminum wiring are less susceptible to deviations in installation practice.
Failure of Nickel Anodes in a Heavy Water Upgrading Plant
Authors: Gill T.P.S. , Gnanamoorthy J.B. , Rangarajan V.
Published: May 2019

Nickel anodes failed in several electrolysis cells in a heavy-water upgrading plant. Dismantling of a cell revealed gouging and the presence of loosely attached black porous masses on the anode. The carbon steel top, plate was severely corroded. An appreciable quantity of black powder was also present on the bottom or the cell. SEM/EDX studies of the outer and inner surfaces of the gouged anode showed the presence of iron globules at the interface between the gouged and the unattacked anode. The chemical composition of the black powder was determined to be primarily iron. Cell malfunction was attributed to the accelerated dissolution of the carbon steel anode top, dislodgment of grains from the material, and subsequent closing of the small annular space between the anode and the cathode by debris from the anode top. Cladding of the carbon steel top with a corrosion-resistant material, such as nickel, nickel-base alloy, or stainless steel, was recommended.
Fatigue Failures of Connecting Bolts in a Truck Crane
Authors: Kitsunai Yoshio , Maeda Yutaka
Published: May 2019

JIS SCM435 steel bolts that connected the slewing ring to the base carrier on a truck crane failed during the lifting of steel piles. The bolts were double-ended stud types and had been in operation for 5600 h. Failure occurred in the root of the external thread that was in contact with the first internal thread in the slewing ring. Examination of plastic carbon replicas indicated that failure was the result of fatigue action. Failure was attributed to overloading during service and increased stress concentration on a few bolts due to nonuniform separations around the slewing ring. A design change to achieve equal separation between bolt holes was recommended.
Termination Delamination of Surface-Mount Chip Resistors
Authors: Runge-Marchese Jude M.
Published: May 2019

Several surface-mount chip resistor assemblies failed during monthly thermal shock testing and in the field. The resistor exhibited a failure mode characterized by a rise in resistance out of tolerance for the system. Representative samples from each step in the manufacturing process were selected for analysis, along with additional samples representing the various resistor failures. Visual examination revealed two different types of termination failures: total delamination and partial delamination. Electron probe microanalysis confirmed that the fracture occurred at the end of the termination. Transverse sections from each of the groups were examined metallographically. Consistent interfacial separation was noted. Fourier transform infrared and EDS analyses were also performed. It was concluded that low wraparound termination strength of the resistors had caused unacceptable increases in the resistance values, resulting in circuit nonperformance at inappropriate times. The low termination strength was attributed to deficient chip design for the intended materials and manufacturing process and exacerbated by the presence of polymeric contamination at the termination interface.
Explosion of an Oxygen Line
Authors: Leeser David O.
Published: May 2019

An oxygen line that was part of a mobile, truck -mounted oxygen-acetylene welding unit exploded in service. Analysis revealed that the failure occurred at the flexible hose-to-valve connection. It was further determined that a steel adapter had been installed at the point of failure to make the connection. Use of the adapter which joined with a brass nipple, created an unacceptable dissimilar metal joint. The steel also provided a source for the generation of sparks. Loctite, a hydrocarbon sealant that is highly flammable and explosive in contact with pure oxygen, had been used to seal the threaded joint. It was recommended that only brass fittings be used to assemble removable joints and that use of washers, sealants, and hydrocarbon lubricants be strictly avoided.
On the taxonomic recognition of skinks from the Guadeloupe Archipelago (Squamata, Mabuyidae, Mabuya)
Authors: Hedges S. Blair , Lorvelec Olivier , Barré Nicolas , Vidal Nicolas , Pavis Claudie
Published: May 2019

The six species of mabuyid lizards (skinks) of the Guadeloupe Archipelago are Capitellum mariagalantae, Mabuya cochonae, M. desiradae, M. grandisterrae, M. guadeloupae, and M. parviterrae. All are critically endangered and four may be extinct, primarily from predation by introduced mammals. These six species were described in recent years from molecular and morphological analyses. Miralles et al. (2017, Bulletin de la Société Herpétologique de France, 163, 67–84) has challenged the taxonomy, claiming that the six species cannot be diagnosed from each other, and recognized only a single species, Mabuya desiradae. We find that their study contains errors that led them to that incorrect conclusion, including a probable data handling error in the molecular analysis and the use of non-diagnostic morphological characters.
Analyse chimique, activités antioxydante, anti-inflammatoire et cytotoxique d’extrait hydrométhanolique d’Origanum glandulosum Desf.
Authors: Krimat S. , Metidji H. , Tigrine C. , Dahmane D. , Nouasri A. , Dob T.
Published: May 2019

L’extrait hydrométhanolique des parties aériennes d’Origanum glandulosum Batt. et Trab. a été étudié pour sa composition chimique par analyse CLHP et ses activités antioxydante, anti-inflammatoire et cytotoxique. L’analyse chromatographique a révélé la présence de trois acides phénoliques et de huit flavonoïdes. Les résultats de pouvoir anti-oxydant qui ont été réalisé par la méthode de DPPH (2,2-diphenyl-1-picrylhydrazyl) et de β-carotène–acide lino-léique indiquent que l’extrait possède une forte activité. Les résultats ont montré aussi que l’extrait de la plante a une excellente activité anti-inflammatoire dans les deux modèles in vivo (l’œdème de la patte induit par la carragénine et l’œdème de l’oreille induit par l’huile de croton). De plus, cet extrait a été trouvé comme possédant une bonne toxicité contre les larves d’Artémia (LC50 = 17,64 μg/ml).